Discussion Chain ID: 32076
================================================================================

User asked: What's the simplest way to etch Nickel and Chromium sputtered layers?

I have to etch a very thin film (50 nm) of Nickel ($\ce{Ni}$) on a 100 nm $\ce{SiO2}$/$\ce{Si}$ substrate. Additionally, there is a ~5 nm adhesion layer of $\ce{Cr}$ under the $\ce{Ni}$ that I'd also like to etch. So I found [this page](http://www.cleanroom.byu.edu/wet_etch.phtml) which has a fairly long list of etches for $\ce{Ni}$ and $\ce{Cr}$. Ni: > > 1 : 1 : 1 - HNO3 : HAc : Acetone > 1 : 1 - HF : HNO3 > 30% FeCl3 > 3 : 1 : 5 : 1 - HNO3 : H2SO4 : HAc : H2O 85 C 10 microns/min > 3 : 7 - HNO3 : H2O > 1 : 1 - HNO3 : HAc > 10% g/ml Ce(NH4)2(NO3)6 : H2O > HF, concentrated – slow etchant > H3PO4 – slow etchants > HNO3 – rapid etchant > HF : HNO3 – etch rate determined by ratio, the greater the amount of HF the slower the reaction > 4 : 1 - HCl : HNO3 – increase HNO3 concentration increases etch rate > 30% FeCl3 > 5g : 1ml : 150ml - 2NH4NO3.Ce(NO3)3.4(H2O) : HNO3 : H2O – decreasing HNO3 amount increases the etch rate > 3 : 3 : 1 : 1 - H3PO4 : HNO3 : CH3COOH : H2O ~15min/micron @ RT with air exposure every 15 seconds > Cr: > 2 : 3 : 12 KMnO4 : NaOH : H2O > 3 : 1 H2O : H2O2 > concentrated and dilute HCl > 3 : 1 HCl : H2O2 > 2 : 1 FeCl : HCl > Cyantek CR-7s (Perchloric based) 7 min/micron (24A/s new) > 1 : 1 HCl : glycerine 12min/micron after depassivation > 1 : 3 [50gNaOH+100mlH2O] : [30g K3Fe(CN)6+100mlH2O] 1hr/micron I'd really like to avoid HF if I can (it terrifies me!), but I have pretty much everything else at my disposal. So far, everything I've done has been at room temperature. First I tried concentrated $\ce{FeCl3}$. No bubbling or signs of anything after ~20min. Then I tried weak $\ce{H3PO4}$. Nothing. Today I tried strong (98%) $\ce{H3PO4}$, nothing. Then I tried concentrated fuming $\ce{HNO3}$. Nothing after ~1hr. Then I tried about 1:1 $\ce{HNO3}$:$\ce{HCl}$, nothing. Am I missing something here? Do the solutions need to be heated up or something?

Discussion:
Comment: I don't know the exact chemistry, but nickel actually etches better in dilute nitric acid than concentrated. Many commercial etchants are just ~15% nitric acid in water with a bit of surfactant added. Heating typically increases the etch rate, but dilute nitric acid should still give you 3 or 4 nm/s at room temperature.
Comment: @MichaelD.M.Dryden, huh, strange. Very counterintuitive to my 8th grade level knowledge of chemistry. I'll try that. Now that you mention it, several of those recipes above call for DI H2O in addition to the acids. I kind of assumed they were actually slowing down the rate, but maybe they're necessary.

Answer 1 (2 votes):
Nickel can be etched using diluted (1:1 V) $HCl$. 50 nm will be dissolved within seconds. The etching solution for the chromium layer contains $\ce{Ce(NH4)2(NO3)6}$+$\ce{CH3COOH}$+$\ce{H2O}$ in ratio 165g : 45 ml (con.) :100 ml DI water. The chromium layer is dissolved within 5 minutes of etching.

Discussion on this answer:
Comment: Hmm, do you mean at room temperature? Because I'm pretty sure I tried the dilute HCl and found it to not work... Cr is easy to etch in my experience, we have a simple commercial acetic acid based one that works well.
Comment: Yes at RT, I did this etching a lot of times. I was etching 200 nm Ni layer by diluted HCl and it worked perfectly well for microstructures preparation on glass. If HCl does not work, then there is something different than Nickel.


================================================================================

